Page:United States Statutes at Large Volume 116 Part 4.djvu/767

 PROCLAMATION 7529-MAR. 5, 2002 116 STAT. 3195 ANNEX (continued) 6 (H) continuous cast cold-rolled drawing quality sheet steel, ASTM a-620-97, Type B, or single reduced black plate. ASTM A-625-92, Type D, T-1, ASTM A-625-76 and ASTM A-366- 96, T1-T2-T3 commercial bright/luster 7A both sides, RMS 12 maximum, with thickness range of 0.22 to 0.97 mm, width of 584 to 937 mm; (I) single reduced black plate, meeting ASTM A-625-98 specifications, 0.148 mm thick, with a temper classification of T-2 (49-57 hardness using the Rockwell 30 T scale); (J) single reduced black plate, meeting ASTM A-625-76 specifications, 0,15 mm thick, MR type matte finish, TH basic tolerance as per A263 trimmed; (K) single reduced black plate, meeting ASTM A-625-98 specifications, 0.18 mm thick, with a temper classification of T-3 (53-61 hardness using the Rockwell 30 T scale); (L) cold-rolled black plate bare steel strip, meeting ASTM A-625 specifications and having the following characteristics: thickness: 0.15 mm +/- 0.008 mm; chemical composition: maximum carbon content of 0.13 percent, by weight; maximum manganese content of 0.60 percent, by weight; maximum phosphorus content of 0.02 percent, by weight; maximum sulfur content of 0.05 percent, by weight; mechanical properties: hardness: T2/hr 30t 50-60 aiming; elongation of greater or equal to fifteen percent; and tensile strength aiming for 352 MPa+/-28MPa; (M) cold-rolled black plate bare steel strip, in coils, meeting ASTM A-623, table ii. Type MR specifications, which meet the following characteristics: thickness: 0.15 mm +/-0.0I3 mm; width of up to and including 254 mm + 9.5 mnV-O; chemical composition; maximum carbon content of 0.13 percent, by weight; maximum manganese content of 0.60 percent, by weight; maximum phosphorus content of 0.04 percent, by weight; maximum sulfur content of 0.05 percent, by weight; mechanical properties: elongation of 15 percent in 50.8 mm, minimum; and tensile strength of 379 MPa maximum; (N) "blued steel" coil (also know as "steamed blue steel" or "blue oxide") with a thickness and size of 0.30 mm x 0.42 mm and width of 609 mm to 1219 mm, in coil form; (O) cold-rolled steel sheet, coated with porcelain enameling prior to importation, which meets the following characteristics: nominal thickness: less than or equal to 0.48 mm; width of 889 mm to 1524 mm; chemical composition: maximum carbon content of 0.004 percent, by weight; minimum oxygen content of 0.010 percent, by weight; and minimum boron content of 0.012 percent, by weight; (P) cold-rolled steel meeting the following characteristics: width: greater than 1676 mm; chemical composition: maximum carbon content of 0.07 percent, by weight; maximum manganese content of 0.67 percent, by weight; maximum phosphorus content of 0.14 percent, by weight; maximum silicon content of 0.03 percent, by weight; physical and mechanical properties: thickness range of 0.800 to 2.000 mm; yield point (MPa) of 265 to 365; minimum tensile strength (MPa) of 440; and minimum elongation of 26 percent; (Q) band saw steel meeting the following characteristics: thickness less than or equal to 1.31 mm; width less than or equal to SO mm; chemical composition: carbon content of 1.2 to 1.3 percent, by weight; silicon content of 0.15 to 0.35 percent, by weight; manganese content of 0.20 to 0.35 percent, by weight; phosphorus content less than or equal to 0.03 percent, by weight; sulfur content less than or equal to 0.007 percent, by weight; chromium content of 0.30 to 0.5 percent, by weight; and nickel content less than or equal to 0.25 percent, by weight; other properties: carbide: fully spheroidized having greater than 80 percent of carbides, which are less than or equal to 0.003 mm and uniformly dispersed; surface finish: bright finish free from pits, scratches, rust, cracks, or seams; smooth edges; edge camber (in each 300 mm of length) of less than or equal to 7 mm arc height; and cross bow (per 25.4 mm of width) of 0.015 mm max;

�